Giant Magnetoresistive (GMR) Sensor Microelectromechanical System (MEMS) Device for Nondestructive Evaluation (NDE) Health Monitoring Applications for International Space Station (ISS) R. Ramesham*,J. D. Olivas', S. Stokes', W. Wilson', and Edward Generazio3 *Jet PropulsionLaboratory, California Institute of Technology 4800 Oak Grove Drive, Pasadena, CA91 109 1 Lyndon B. Johnson Space Center, 2101 NASA Road1, Houston, TX 77058 2 Rice University, Houston, TX 77005 3 Langley ResearchCenter, Hampton, VA2368 1-2199 ABSTRACT With the imminent launch of the first International Space Station modules, NASA Oflice of SafetyandMissionAssurance,specifically the Code Q Nondestructive Evaluation Program, is addressing issues of on-orbit station structural health monitoring. Aspart of thiseffort, Jet Propulsion Laboratory isworkingwithNASA'sLangley Research Center ondevelopment of noveldevicesand sensors for an NDE tool kit intended to beused by Space Station Astronauts for non-intrusive structural health assessment. JPL is currently investigating applicability of giant magnetoresistive technology, originally developed for high-density magnetic media, married to state of the art microelectromechanicalsystems (MEMS) for application as an acoustic sensor. In addition to spaceapplications, these deviceswouldhavewidespreadapplicability in earthbound environmentssuch as continuoudintermittent healthmonitoring of aircraft, hazardous process machinery and manyother applications. This paper discusses the fabrication aspects of a sensor device that is based on a sputter deposited, multilayer, giant magnetoresistive field sensor. The device consists of a micromachined microstructure (membrane, cantilever beam, bridge) and a sputtered hard magneticfilm. The device detects acceleration by sensingchangesinmagneticfield caused by the displacement of the hard magnetic film on the microstructure. Utilizing the bulkmicromachining approach, verythin (0.5 - 1 pm) siliconandsiliconnitride membranes are fabricated by means of anisotropic etching of silicon wafers and/or reactive ion etching of silicon on insulator (SOI) or Low Pressure Chemical Vapor Deposited (LPCVD) siliconnitridefilms over silicon substrate. The primaryobjective of our program is to study spin valvestructures (giant magnetoresistancein magnetic multilayers) and microelectronics fabrication issues in devices that exhibit the large magnetoresistive effect. Areliable G " E M S deviceshouldhave the followingcharacteristics;a significant percentage change in resistance, high field resistance, low resistance noise, and a high bandwidth. These characteristics are very sensitive to the thickness of the various layers in device multilayers, the composition and microstructure of the individual layers. The eventual goal of our project is to optimize the giant magnetoresistive behaviorof the device using a design of materials approach. Deposition and patterning of hard magnetic film over the microstructure and the bonding of microstructure over the GMR element are
discussed. We also present the fabricationandreliabilityissuesassociatedwithGMR devices. Introduction
The measurement of acceleration has been accomplished using several technologies inhigh-reliabilityapplicationssuch as guidance control, detonation, and shockandvibrationmeasurement.Electromechanical,piezoelectric,piezoresistive,and capacitiveacceleration sensors are available and the literature pertinent to giant magnetoresistive sensors for the above applications are scanty. All accelerometers require the conversion of acceleration into a force, causing a displacement, which is then turned into an electrical signal. This displacementis resisted by a calibrated springof some kind.
F = ma F=-kX a=-kdm
1 2 3
Where F = force, m = Mass, a = Acceleration, k = spring constant, and x = displacement. Equations describing accelerometers are simple and well known. Accelerometers measure “a” by knowing“k” and “m”, observing “x” and using equation 3 above. The GMR effect was discovered in perfect-crystal samples exposed to very high fields.[l] The giant magneto resistive effect was recently discovered in sputtered metallic thin films consisting of magnetic layers a few nanometers thick separated by equally thin nonmagnetic layers. Large decrease in the resistance of these films is observed when a magneticfield is applied.The cause ofthiseffectis the spindependence of electron scattering and the spin polarization of conduction electrons in ferromagnetic metals. With layers of the proper thickness, adjacent magnetic layers couple antiferromagnetically to each other with the magnetic moments of each magnetic layer aligned antiparallel to the adjacent magnetic layers. Conduction of electrons, spin polarized in one magnetic layer with antiparallel conduction electron spins. Frequent scattering of electrons results in high electrical resistivity of the GMR device. If an external field overcomes the antiferromagneticcouplingitachievesparallelalignment of moments in adjacent ferromagnetic layers; the spin dependent scattering of conduction electrons is decreased and resistivity decreases. The size of this decrease in resistivity can be 10% to 20% and higher in GMR materials with multiple nonmagnetic layers. [2,3] The primary advantage of GMR materials is greater sensitivity to magnetic fields. This increased sensitivity makes it possible to detect smaller change in the magnetic fields. Large signals from GMR materials structures also help overcome electronic noise. The difference between magnetoresistive (MR) and GMR sensors is sensitivity, measured by percent change in resistance. In a M R sensor a resistance change is causedby the intrinsic is caused by the property of the sensinglayer.InaGMRsensoraresistancechange quantum nature of electrons. [2-41
GMR sensors are composed of four thin films suchas a sensing layer, aconducting spacer, a pinned layer, and an exchange layer. The thickness of all the layers is very thin except for the exchange layer which will allow the conduction of electrons to frequently move back and forth between the sensing and pinned layers via the conducting spacer. The magnetic orientation of the pinned layer is fixed and held in place by the adjacent exchange layer, whilethe magnetic orientation of the sensing layer changes in responseto the external magnetic field. A change in the magnetic orientation of the sensing layer will cause a change in the resistance of the combined sensing and pinned layers. GMR sensor materials havetwo spin directions known as spin up and spin down. Conduction electrons with a spin direction parallel to a material’s magnetic orientation move freely, producing low resistance.Conversely,conduction electrons withspindirection opposite to the materials magnetic orientationare hampered by more fiequent collisions with atoms in the material, producing higher resistance.  GMR sensors directly detect the magneticfieldandthey are sensitive to small changes in the magnetic fields, and they can be used to measure position or displacement in linear and rotational systems. Some of the applications for GMR magnetic sensors are current sensing, linear or rotatory motion detection, linear or rotatory position sensing, ignition timing, throttle position sensing, etc.  GMR sensors have greater output than conventional anisotropic magnetoresistive sensors. Principle of operation: The magnetic field H adjacent to hard magnetic thin film will hold the following relationship:
Where a is the constant of order, h is the average distance between domainsin the magnet and d is the distance between the GMR sensor and the hard magnetic thin film which certainly depends onthe acceleration.
Experimental Details DC magnetron sputtering has been used to sputter multilayers in a UHV chamber. The silicon dioxide has beengrown over silicon, which was usedas substrate in this study. The sputtering was performed at room temperature and at an argon ambient. The silicon dioxide/silicon substrate was mounted away from the target in the vacuum chamber. The structure of a typical spin valve is siliconhilicon dioxide/tantalum/copper/cobalt/ FeMn/ Tantalum. Changing the layer thickness changesthe magnetic coupling between the layers and cobalt layer is inserted between the permalloy and copper to boost the GMR ratio and keep the permalloyfrommixingwith the copper. Carbon oxygen impurities have been shown to reduce GMRperformance.Table 1 shows the typicaldepositionparameters employed to deposit GMR device stack layers by magnetron sputtering technique. We have analyzed the GMR device structure with energy dispersive x-ray analysis(EDAX) to [email protected]
the elementspresent in the stack of GMR.Identified all the elements as anticipated withEDAX analysis. 3
Issues relating to GMR sensor fabrication: Controllingthe thickness of the copper spacer layer, temperature stability, electrostatic discharge, change in magnetization, lift off technique approach, annealingofhardmagneticthinfilm,and the fielddamagewill influence the GMR characteristics. Issues associatedwith the reliability of GMR sensors are thickness control of the copper spacer layer. The other critical issue is the temperature stability.Theproduction of spinvalvesusesan IrPtMn antiferromagnetic layer as a pinning layer for the spin valves. This layer can withstand cycling above 350°C. Cobalt and copper do not mix at moderate temperatures, however permalloy and copper do mix and if permalloy is used adjacent to copper, the spin valve will degrade around 200°C. GMR layers are extremely thin, only about 300 - 400 & so the temperature rise froma voltage spikecanmelt the layers. There isalso danger of the magnetization changingif the temperature of the layerexceeds the Nee1 temperature of the GMR materialshouldhaveresistance to electrostatic antiferromagneticlayer.The discharge and resistance to thermal degradation. The GMR element may be characterized by its change in resistance AR/R when the field changes by an amount of AH. The ratio of AWAH may be in the range of 0.1 WOersted. The objective in making this device is to measure to a typical distance, which is in the order of 1 nm. The sensitivity and response time of the mechanicalassemblywilldepend on the couplingbetween the membrane (moving microstructure) and the GMR element. The maximum response time will be in the range of 10 - 0.2 psec for 1 nm displacement of moving part. A dogbone structure has been used to fabricate magnetoresistive GMR element that has a resistance, R that depends on the local field, H at the GMR sensor. If the resistance is usedto.measure field of the hnction H intensity the displacement “d” may be determined with a simple inversion as described in eqn. 4. [6-81 Fabrication of GMR sensor: The fabricationof GMR sensor involves three steps and they are as follows: 1 . Fabrication of GMR sensor on the substrate, 2. Fabrication of the movable microstructure such as a membrane or a cantilever beam, or a bridge and finally, 3. Deposition of hard magnetic thin film on the movable microstructure. Critical issues associated with the fabrication of a GMR sensor device are signal to noise ratio, geometry andlithographicdefinition of the spinvalveon the substrate, magnetic properties of hardmagneticthinfilm,and process integrationwith surface andbulk micromachining processes. Patterning of spin valve: The GMR elementmaybefabricatedusingseveral layers of various metallic thin films patterned by using photolithography. Patterning of GMR element can be achieved by hydrochloric acid plasma,lift-off technique, ion milling, or chemical etching. Chemical etching may not yieldfruithl results of patterning since the GMR element consists of various multi layers that could form galvanic couples in the chemical solutions. Different layers can be etched at differentrates in the chemical etching solutions due to the galvaniccoupling.Wehaveusedasingle step self-aligned photolithographic lift-off techniqueto attain the patterning of GMR elements in this study. There may be some technical problems associated with the poor edge definition of GMR
elements in the lift-offtechnique.Therefore,experimentsusingHClplasmaand milling will be planned shortlyto attain GMR element fabrication.[101
Possible hard magnetic thin film materials: A hard magnetic thin film element will be depositedover the moving microstructure (membrane, cantilever beam, or a bridge ) and patterned using an appropriate technique. The lift-off technique may be used to pattern the hardmagneticthin film. Adhesionwillbeimproved by depositing Cr by magnetron sputtering. Co-sputtering of CoCrTaPt will be deposited by lift-off technique. There is no wet etching solution available to pattern CoCrTaPt, FePt, Copt to act as a hard magnetic thin film.  Fabrication of moving microstructure: A moving microstructure of silicon, silicon nitride, or silicon dioxide may be fabricated using various approaches. A silicon membrane may be fabricated usinganisotropic etching of silicon using silicon nitride mask and a potassium hydroxide solution. It is very difficult to fabricate a silicon membrane of 1 pm or less using this chemical etching solution approach. A silicon membrane may also be fabricated using a plasma-etching approach. Deep reactive ion etching technique has been used to etch the silicon substrate at a rate of 5 - 10 pdmin. Aluminum can be used as a mask to fabricate silicon membranes. It has been observed in our study that there will be a micromasking effect with aluminum in the R E etched area. Thick photoresist has been used as a mask to etch silicon by RE to fabricate silicon membranes.[1 1-13] It is difficult to fabricate 1 pm or less thick silicon membranesby RIE since the etching rate is significantly high. Therefore, an alternative approach could be silicon on insulator (SOI) substrate to fabricate silicon membranes. One may etch silicon either by RIE or chemical etching solutions. It is possible to fabricate 3 -5 pm thick silicon membranes. However, we need 1 pm or lessthicksiliconmembranes to use as amoving microstructure to implement in the GMR sensor device. Finally, we have chosento fabricate a silicon nitride membrane,whichisapparentlyquitestableinKOHsolutions.Siliconnitridehasbeen grown on both sides of a silicon substrate using low-pressure chemical vapor deposition (LPCVD). The Si3N4 was patterned and then plasma etcheddown to the silicon substrate. The silicon substrate was etched in KOH solution untilthe other silicon nitride is reached. Thus 0.5 pm silicon nitride membranesare fabricated over silicon substrates.
Results and Discussion Figure 1 shows the schematic of the completegiantmagnetoresistive (GMR) accelerometer device. This complete device may be fabricated over two silicon chips and finally may be bondedby an appropriate technique. A silicon substrate has been chosen in this studyandsiliconnitridewasdepositedusingLPCVDtechnique. One side of the silicon substratehilicon nitride was completely etched utilizing either plasma etch or hot phosphoric acid etch solution, while protecting the silicon nitride on the other side of the silicon substrate. Thermally grown silicon dioxide may be grown on the silicon substrate where silicon nitride was etched. The oxide is patterned and etched in the buffered oxide etch (BOE). The hard magnetic thin film was deposited and patterned over the moving microstructure. Siliconnitrideon the other side of silicon substrate was patternedand
plasma etched down to the silicon substrate. The hard magnetic thin film was protected and (anisotropy) chemically etched siliconsubstrate all the way until the silicon nitride thin film. This has produced the moving microstructure with a hard magnetic thinfilm pattern. Another silicon substrate may be chosen and the growth of silicon dioxide was performed by thermaloxidation.Giantmagnetoresistiveelement will befabricatedusing lift off technique on the silicon dioxide. These two chips will be bonded using anodic bonding or any other appropriate technique to assemble the device as shown inthe Fig. 1. [141 Figure 2 shows a scanning electron micrographof the anisotropically etched silicon membrane. LPCVD silicon nitride has been used as a mask to etch silicon substrate and subsequently to fabricate the siliconmembrane.This approach seems to bedifficult to fabricate a silicon membrane of 1 pm or less thick. We have successhlly fabricated a 0.5 pm LPCVD silicon nitride membraneto fabricate the eventual device as shown in the Fig. 1. Figure 3 shows the schematic diagram of the GMR element fabrication. A silicon substrate has been chosen and oxidized by thermal oxidation. The photoresist was spin coated andpatternedusingphotolithography.Tantalum was deposited for electrical contact and to isolate the permalloy from the silicon dioxide. A sensing layer of permalloy was depositedandsubsequentlycobalt, copper, cobalt,iron-manganese,andfinally tantalum were deposited in the same deposition set-up using the same vacuum chamber. Cobalt was deposited to separate the mixing of permalloy and copper and also the mixing of iron-manganese and copper. Copper is deposited to act as a spacer in this device. The top tantalum layer is deposited to protect the device from oxidation and contamination with other impurities. 14-17] Figure 4a shows the scanning electron micrograph of the fabricated GMR device over the silicon dioxide/silicon substrate using lift-off technique. Figure 4b and 4c are the magnified views of the single GMR element and acomer of the GMR element. Figure 5af show the scanning electron micrographs of the GMR element in various regions of the device, Thelift-offtechniqueemployed in this experimenthasyielded poor edge definition. We feel that, this might effect the anticipated sensor response results. During the growth of GMR stack, a magnetic field is applied to the sample to induce easy and hard axesin the magnetic layers and set the direction for the pinning field in the antiferromagneticlayer. In operation the magneticfield to besensed is applied parallel to the hard axis since there is very little hysteresis along this direction and the response is linear for small changes in field. Figure 6 is a plot of the resistance change versus the field applied along the hard axis. The resistance changed by about 3.9 % over the entire field range. There are some issues with the liftoff that lead to a less than ideal GMR curve in Figure 6 . Specifically, any surface contamination leftafter the development of the photoresist will result in rough layers. Rough or wavy interfaces in GMR device increases the ferromagnetic coupling between the two magnetic layers. Also, if the walls of the resist were not perfect additional magnetic coupling could arise.
Figure 7 shows the power versus the frequency whenan ac field was applied to the GMR device along with a dc bias field of 15 Oe. The magnitude of the field applied in Fig. 7 was 0.6 Oe (500 Hz sine wave) and the current through the device was 6 mA (device resistance is about 480 K). The absence of higher harmonic peaks indicates that there was little distortion and an output of pure sine wave. The baseline noise in Fig. 7 is due to intrinsic l/f noise in the spin valve. l/f noise is the dominant noise source until about 20 KHz depending on the current, at higher frequencies thermal noise is dominant. The magnitude of the l/f noise increasesas the square of the current. Table 1 shows the some of the experimental spin valve configurations that have been tested in the laboratory at Rice University. Adding the cobalt layer in the GMR device structure has significantly improvedthe device characteristics. Further experiments are underway to understand the significance of the various layers. Table 1: The change in resistance as a function of spin valve configuration  Device #
1 2 3
Co/Cu/Co/FeMn NiFe/Cu/NiFe/FeMn NiFe/Co/Cu/Co/NiFe/FeMn
Table 2 shows the test results on the some of the GMR devices fabricated at the Rice University. The change in resistance was high (6.3%) when there is thick cobalt layer and also the permalloy layer was absent. A permalloy layer has been incorporated in the device 2 andcobaltlayerthicknesslayerhasbeenreduced to 15 A. The change in resistance has reduced to 4.5%. The cobalt layer has been completely eliminated in the device 3 and the changeinresistancehasbeenreduced further. The copper layer thickness isdifferentfrom the criticalthicknessrequired to obtainhighchangein resistance. Further experiments are underway to characterize the GMR devices. Table 2: GMR Device Test Results
1 2 3
64 50 50
44 44 44
80 80 80
64 50 50
6.3% 4.5% 1.6%
We have used the appropriate layers such as sensing layer, conducting spacer and antiferromagnetic layer andother space layersto avoid the mixing of the sensing layer and
conducting spacer. Identified the problems associated with the fabrication of verythin siliconmembranesand we havefabricated 0.5 micronlowpressurechemical vapor of siliconand depositedsiliconnitridemembranesusinganisotrpicchemicaletching plasmaetching of siliconnitride.Identified the hardmagneticthinfilm,whichwillbe deposited over the moving silicon nitride microstructure to demonstrate the GMR sensor device.We willshortlybeassembling the GMRdevices,hardmagneticthinfilm fabricated over moving silicon nitride microstructure components using, and appropriate process to characterize the sensor response characteristics. Acknowledgments
This researchwork was carried out at the Jet Propulsion Laboratory, California Institute of Technology and Rice University andwas supported by NASA. Thanks are due to Mr. Stephen R. Bolin for his constructive comments onthe manuscript. References
1. M. N. Baibich, J.M. Broto, A. Fert, F. Nguyen Van Dau, F. Petroe P. Etienne, G. Creuzet, A. Friederich, and J. Chazelas, Phys. Rev. Lett., 61 (1988) 2472. 2. S.P. Parkin,“GiantMagento-resistance in sputteredmagneticsuperlattices”, 35* Annual conference on magnetism and magnetic materials, November 27 - December 4, 1989. Abstract was published in Journal of Applied Physics, 67, 593 1(1990).
3. Nonvolatile Electronics Inc., Engineering& Application Notes, http://www.nve.com. 4.P.
Grunberg,“Magnetic field sensorwithferromagneticthin filmlayershaving magnetically antiparallel polarized components,”U.S. Patent, 4,949,039.
5. B. *A. Gurney, V. S. Speriosu, D.R. Wilhoit, H. Lefakis, R.E. Fontana, Jr., “Can spin valve be reliably depositedfor magnetic recording?’, J. Appl. Phys., 81 (1997) 3998.
6. S. Mao, N. Amin, and E. Murdock, J. Appl. Phys., 83 (1998) 6807. 7. A. Wallash, Data Storage, Test and Measurement, January 1998, p. 37. 8. J. Szucs, T. O’Brien, and D.K. Lottis, S. Gangopadhyay, S. Mao, and E. Murdock, J.
Appl. Phys., 81 (1997) 4014. 9. R.J. M. van de Veerdonk, P.J. Belein, K.M. Schep, J.C.S. Kools, M.C. de Nooijer, M.A. Gijs, R. Coehoorn, W.J.M. de Jonge, J. Appl. Phys., 82 (1997) 6152. 10. M. Xiao and M.H. Kryder, Electrochemical Society Proceedings, Proceedings Fourth InternationalSymposiumonMagneticMaterials,processesandDevices,
Application to storage and microelectromechanical systems (MEMS), Edited by L.T. Romankiw and D. A. Herman, Jr., Vol. 95-18, p. 51 (1995). 1 1 . C. D. Ellis, Aburn University, Personal communication, Jan1998. 12. R. Ramesham, C.D. Ellis, J.D. Olivas, and S. Bolin, Thin Solid Films, “Fabrication of diamondmembranes for MEMSusingreactiveionetching of silicon,”ThinSolid Films, 1998. (In Press). 13. Marc Madou, Fundamentals of Microfabrication, CRC Press,New York, 1997.
14. W.F. Egelhoff, Jr., P.J. Chen, C. J. Powell, M.D. Stiles, R.D. McMichael, C.L. Lin, J.M. Sivertsen, J.H. Judy, K. Takano, A.E. Berkowitz, T.C. Anthony, and J.A. Brug, J. Appl. Phys., 79 (1996) 5277. 15. V.S. Speriosu, J.P. Nozieres, B.A. Gurney, B. Dieny, T.C. Huang,and H. Lefakis, Physical Review B, 47 (1993) 11579.
16. J.P. Nozieres, V.S. Speriosu, B.A. Gureny, B. Dieny, H. Lefakis, and T.C. Huang, J. Magnetism and Magnetic Materials,12 1 (1 993)3 86. 17 B. Dieny, J. Magnetism and Magnetic Materials, 136 (1994) 335.
5' s 0
r 3 01 CD
rc r CD
F i e